Scientific Journal of Impact Factor (SJIF): 5.71
e-ISSN (O): 2348-4470 p-ISSN (P): 2348-6406
International Journal of Advance Engineering and Research Development Volume 5, Issue 02, February -2018
Influence of potassium chloride doping on the properties of urea succinic acid single crystals S.K. Amjath Kudos1, A.C. Sajikumar 2, C. Krishnan 3 1
Research Scholar, S.T.Hindu College, Nagercoil , Tamil Nadu, India Department of Physics, Christian College, Kattakada, Trivandrum, Kerala, India 3 Department of Physics, Arignar Anna College, Aralvoimoli, Tamil Nadu, India.
Abstract â€”An organic single crystal of potassium chloride doped Urea Succinic Acid (USA) was successfully grown by slow evaporation technique. The grown crystal was characterized by X-ray diffraction (XRD) which confirms the lattice parameters. FTIR spectral studies were performed to identify he vibrations of functional groups. TGA/DTA studies revealed the thermal stability and the mechanical strength of grown crystal. The UV- vis spectral study reveals the enhancement optical property of grown crystal. Keywords-Crystal Growth, XRD, FTIR, UV, Thermal studies. I.
Many organic crystals have been found potential applications in nonlinear optics and have more application in telecommunication, frequency mixing, optical parametric oscillation, optical bi stability, optical image processing and under water communication etc.[1-3]. The organic NLO materials have large dipole moment, spiral structure, high nonlinear figure of merit for frequency conversion, high laser damage threshold and fast optical response time as compared with inorganic materials . Urea [(NH2)2CO] is one such efficient organic non linear crystal. It is used for high power laser frequency shifting in a wide spectral range because of its large transparency window, large birefringence, relatively high damage threshold and low temperature dependence of the refractive indices. Succinic acid is used as a biodegradable polymer and biological production by fermentation has been focused as the alternative to petro chemical process [5-6]. The growth of succinic acid and urea succinic acid (USA) [7-9] crystals and their properties have been investigated earlier. In the present study, potassium chloride doped with urea succinic acid crystal has been grown by the conventional slow evaporation technique. Attempts have been made to study the characterization of the grown crystal through powder XRD, FTIR, UV, and TGA. II.
The title compound was synthesized by taking urea and succinic acid in a molar ratio of 1:1 and is dissolved in deionized water. Then 2 M percentage dopant potassium chloride solution is added slowly. The solution was agitated with a magnetic stirrer for 6 hours continuously and filtered. The solution was allowed to evaporate at room temperature. After three weeks of grown period, a colorless transparent crystal has been harvested. The photograph of the grown KCl doped USA crystal is shown in Fig. 1.
Fig.1: Photograph of KCl doped USA crystal @IJAERD-2018, All rights Reserved
International Journal of Advance Engineering and Research Development (IJAERD) Volume 5, Issue 02, February-2018, e-ISSN: 2348 - 4470, print-ISSN: 2348-6406 III. CHARACTERIZATION The USA crystal doped with potassium chloride has been subjected to powder X-ray diffraction studies by using X’pert pro powder X-ray diffractometer with Cuk radiation (=1.5418Å). FTIR spectrum was rewarded in the range of 400-4000 cm-1 employing Brukel IFS-66V spectrometer using KBr Pellet technique. The optical absorption spectra of the grown crystals were recorded in the range of 100-1100nm using Varian Carey 5E Spectrophotometer. Thermal stability and decomposition stages were analyzed by recording TGA/DTA spectrum (TGA Q 500 V 20.10 Build 36 thermal analyzer) in the temperature range of 30-800c in nitrogen atmosphere at a heating rate of 20c/min.
3.1. XRD Analysis The well defined Braggs peaks at specific 2 angles have shown high crystalline nature of USA crystal doped with KCl. The intense peaks of the observed powder XRD pattern has been compared with the standard XRD pattern of the reported literature and indexed hence the dielectric constant decreases gradually. The observed powder XRD pattern of the grown crystal is shown in Fig. 2. It is noted that the doped USA crystals are nearly identical with pure USA with some slightly shifting of some intensities which proved that the dopant entered into the crystal matrix of USA .
2 Theata (degrees) Fig. 2: PXRD pattern of KCl doped USA crystal 3.2. FTIR Analysis FTIR spectrum is used to find out the functional groups present in the compound. The observed FTIR spectrum of the grown USA crystal doped with KCl is shown in Fig. 3. The O-H symmetric stretching bond of water occurs at 3480 cm-1 confirms the pressure of water in the crystal. The medium intensity peaks obtained at 3340 and 3230 cm-1 is due to asymmetric and symmetric stretching of N-H. The very strong bands at 2540 and 1700 cm-1 were associated with CH2 and C=O stretching @IJAERD-2018, All rights Reserved
International Journal of Advance Engineering and Research Development (IJAERD) Volume 5, Issue 02, February-2018, e-ISSN: 2348 - 4470, print-ISSN: 2348-6406 respectively. The appearance of medium intensity bands at 1310 and 1020 cm-1 have been assigned to symmetric stretching vibration of C-C and C-N. The presence of carbonyl group has been confirmed by the appearance of the band at 1420 cm -1 in USA crystal doped with KCl. In the present investigation, sharp peak at 901 cm-1 assigned most probably due to O-H out of plane vibration. The rocking mode of NH2 and COOˉ are wagging mode of COOˉ are expected at 800, 442 cm-1 and 571 cm-1 respectively. The FTIR spectrum also shows the high transmission which is used in NLO application .
571 442 636
2750 2640 2540
1420 1310 1200
60 3480 3340 3230
Wavenumbers (cm-1) Fig. 3: FTIR spectrum of KCl doped USA crystal 3.3. Thermal analysis The thermo gram and differential thermo gravimetric (TGA/DTA) traces of KCl doped USA crystal is shown in Fig. 4. In TGA, there is no weight loss up to 140 oC. This indicates that there is no inclusion of water in the crystal lattice. It is found that the first stage of decomposition starts at 140C and ends at 166C with a weight of 32% due to the removal of succinic acid . The second stage (168C-217C) is associated with a weight loss of 62% due to the release of gaseous product NH2, CO etc. The strong endothermic peak at 217.29C in DTA curve corresponds to the melting point of the grown crystal. The prolonged heating beyond 217C up to 343C with a minor weight loss of 3% is due to removal of residual substances. In the DTA curve at 166.08C a phase change is occur, maybe due to the change from ferro electric phase to para electric phase which may be used for Electro optic devices .
@IJAERD-2018, All rights Reserved
International Journal of Advance Engineering and Research Development (IJAERD) Volume 5, Issue 02, February-2018, e-ISSN: 2348 - 4470, print-ISSN: 2348-6406
-0.6 2 -0.8 1
-1.0 -1.165 mg/min
Derivative weight (mg/min)
Temperature (oC) Fig. 4: TGA/DTA Thermograms of KCl doped USA crystal 3.5. Optical studies The optical studies absorption spectrum nm of the USA crystal doped with KCl is shown in Fig.5. It is seen from the absorption spectrum that the crystal is transparent in the entire near UV and visible region (220 nm to 1100 nm). It has been found that the UV cut off wavelength is 219 nm. The low percentage of absorbance in the entire visible region is a desirable property for NLO application .
Wavelength (nm) Fig. 5: Absorption spectra of USA crystal doped wih KCl @IJAERD-2018, All rights Reserved
International Journal of Advance Engineering and Research Development (IJAERD) Volume 5, Issue 02, February-2018, e-ISSN: 2348 - 4470, print-ISSN: 2348-6406 IV. CONCLUSION In the present study the USA crystal, doped with potassium chloride has been grown by the conventional slow evaporation technique. The identity of the crystal has been confirmed by powder XRD techniques. The functional groups presented in the synthesized compound have been verified by FTIR studies. The UV cut off wavelength is found out as 219 nm. The melting point of the grown crystal is to be found out as 217.18C. All characterization properties revealed the NLO application of grown crystal. References  A. Shanthi, B. Krishnan and P. Selvarajan, “Studies on growth and characterization of a novel nonlinear optical and ferroelectric material – N,N-dimethylurea picrate single crystal”, J. Cryst. Growth., vol.393, pp.7-12, 2014.  K. Ambujam, K. Rajarajan, S. Selvakumar, J. Mahadevan, Gulam Mohamed and P. Sagayaraj, “Growth and characterization of an organometallic nonlinear optical crystal of manganese mercury thiocyanate (MMTC)”, Opt.Mat., vol.29, pp.657-662, 2007.  K. Meera, R. Muralidharan, R. Dhanasekaran, P. Prapun Manyum and P. Ramasamy, “Growth of nonlinear optical material: L-arginine hydrochloride and its characterization”, J. Cryst. Growth, vol.263, pp. 510-516, 2004.  D. Shanthi, P. Selvarajan and S. Perumal, “Growth, SHG, THG and Impedance Analysis of Urea. Admixtured L-Alanine (ULA) Single Crystals”, Chem. Tech. Res.,vol.6, pp. 5329-5334, 2014.  M. K. Jain, R. Datta, J. G. Zeikus “ High value organic acids fermentation emerging process and products”, The first generation chichester: Ellis Harwood Press, 1989.  Jiann-Min Chang, Ashok K. Batra, Ravindra B. Lal, “Growth and Characterization of Doped TGS Crystals for Infrared Devices”, Crystal Growth & Design, vol.5, pp.431, 2002.  S. Krishnan, R. C. Justin, S. Krishnan, C. Justin Raj, R. Robert, A. Ramanand, S. Jerome Das, “Growth and characterization of succinic acid single crystals”, Cryst. Res. Tech., vol.42, pp.1087, 2007.  R. Docherty, K. J. Roberts, “Modelling the morphology of molecular crystals; application to anthracene, biphenyl and βsuccinic acid”, J. Cryst. Growth., vol.88, pp.159,1988.  C. Justin Raj, S. Dinakaran, S. Krishnan, B. Milton Boaz, R. Robert and S. Jerome Das, “Studies on optical, mechanical and transport properties of NLO active L-alanine formate single crystal grown by modified Sankaranarayanan– Ramasamy (SR) method”, Opt. Commun., vol.281, pp.2285-2290, 2008.  S. K. Geetha, R. Perumal, S. Moorthy Babu and P. M. Anbarasan , “Habit modification and improvement in properties of potassium hydrogen phthalate (KAP) crystals doped with metal ions” Crystal Research and Technology, vol.41, pp.221-224, 2006.  N. N. Shejwal, S. S. Hussaini, Ramesh B Kamble, M. D. Shirsat, “Studies on the Structural, Thermal, Fluorescence and Linear–Non-linear Optical Properties of Glycine Sodium Acetate Single Crystal for Electro-Optic Device Applications”, Recent Trends in Materials Science and Applications, vol.2, pp.493-501, 2017.  S. R. Suthar, S. J. Joshi, B. B. Parech and M. J. Joshi, “Dielectric study of Cu2+ doped calcium tartrate tetrahydrate crystals” Ind. J. Pure and App. Phys., vol.45, pp.48-51, 2007.
@IJAERD-2018, All rights Reserved